Of brass and bronze in prehistoric Southwest AsiaChristopher P. Thornton
ABSTRACT This paper presents a review of the numerous copper-zinc alloys (e.g. brass, gunmetal) that have been found in prehistoric contexts from the Aegean to India in the 3rd to the 1st millennium BC. Through a preliminary analysis of the available data, it is argued that there is a noticeable geographical and chronological correlation between early occurrences of copper-zinc alloys, tin-bronze, and rare examples of tin and tin-based metals. This association may have important implica-tions not only for research into the great tin question of Southwest Asia, but also for research into ancient technologies in general. It is here proposed that brass may have been confused with tin-bronze by local consumers ignorant of or ambivalent about the very different mechanical properties of these two alloys, and that the linguistic separation of these two metals in the 1st millennium BC may reflect larger changes in the sociocultural categorisation of materials.
Keywords: brass, tin-bronze, gunmetal, Near East, colour, symbolism, ethnocategories.
The alloys of copper and zinc, including brass (copper-zinc), gunmetal (copper-tin-zinc), and variants thereof, have never played a significant role in our understanding of Old World prehistory (Fig. 1). This is due in large part to their purported absence, or at best sporadic existence, in archaeological assem-blages before the Greco-Roman period (Bayley 1998). Indeed, the origins of copper-zinc alloys have long been placed in Anatolia during the early 1st millennium BC (see Craddock 1978a; Forbes 1964: 2689) an assumption supported by and somewhat predicated on the discovery of early brass artefacts inside the Great Tumulus at the Phrygian capital of Gordion (Steinberg 1981). The fact that this tomb, labelled MM or Midas Mound, was supposed to hold the remains of
the mythical king led Dorothy Kent Hill (1969: 61) to famously suggest that perhaps the story of Midass golden touch in fact referred to the earliest production of brass i.e. turning copper into gold.
This narrative for the development of copper-zinc alloys in Southwest Asia has gradually changed as more examples of these yellow- or golden-coloured metals have been found, both in reviewing the available literature and through further analyses. As recent papers have shown, copper-zinc alloys occur sporadically in this region as early as the 3rd millennium BC, and continue to appear intermittently until the Greco-Roman period (Craddock and Eckstein 2003; Thornton and Ehlers 2003). Having established the existence of copper-zinc alloys in prehistory, we are left with a number of pressing questions including: where are the ancient textual references to the production of brass or gunmetal or to their distribu-tion? Why do we discover only a few copper-zinc alloys in random sites separated by thousands of kilometres despite the innumerable prehistoric artefacts that are analysed every year? Should we care, or can we simply dismiss these sporadic occurrences of copper-zinc alloys as occasional acts of tech-nological serendipity?
In this paper, an up-to-date (i.e. prior to 2006) compila-tion of prehistoric copper-zinc alloys in Southwest Asia is presented in six general chronologically and spatially defined groupings in an attempt to answer these questions. Although these groupings are based on limited data, they provide us with a new perspective on the where, when and how of early brass and gunmetal exploitation. Using these data, it is argued that there is a notable correlation between the occurrence of these rare metals and the appearance and utilisation of tin-bronze, a metal that (unlike brass) has figured prominently in discussions on the development of urban civilisations in western Asia (e.g. Franklin et al. 1978; Muhly 1973; Parzinger and Boroffka 2003; Penhallurick 1986; Pernicka 1998; Stech and Pigott 1986; Weeks 1999). Indeed, it is proposed that by
Figure 1 Ternary diagram showing the standard nomenclature for copper-zinc-tin-lead alloys (from Bayley 1998).
C H R I S TO P H E R P. T H O R N TO N
studying ancient copper-zinc alloys, we may gain not only a richer understanding of the production and utilisation of different materials in prehistoric societies, but also discover a new avenue of research into the classic question on the origins of Near Eastern tin and tin-bronze first posed over 75 years ago by V. Gordon Childe (1928). For this reason, it is suggested that copper-zinc alloys are perhaps of greater importance than has long been assumed, and should begin to receive the scholarly attention that they are due.
Before delineating the six general groupings mentioned above, it is important to understand the basic processes through which copper-zinc alloys could have been produced in antiquity. As numerous scholars have argued, the production of copper-zinc alloys is more complicated than the creation of other copper-based alloys (Craddock 1998a; Pollard and Heron 1996: 196204). This is due to the volatility of zinc above 906 C, which is below the temperature at which zinc will reduce from its ores. Thus any attempt to smelt zinc ores causes zinc to sublimate (vaporise) (Forbes 1964: 263). Under extreme reducing condi-tions the gaseous zinc will condense along the inner wall of the furnace as zinc metal a process known as distillation. If air is present and most ancient furnaces were not designed to be completely airtight then the zinc vapour condenses along the inner furnace lining in the form of zinc oxide (calamine). Given that distillation apparatuses capable of producing great quantities of metallic zinc were virtually unknown (or at least unused) before historical periods, the zinc had to be added either as a vapour to solid copper through a process known as cementation, or through a specially controlled mixed smelt-ing of zinc and copper oxides. While the actual mechanism through which zinc enters the copper is essentially the same for the two processes, the outlook and the set of choices made by the metalworker is inherently different.
The crucial ingredient in both processes is zinc oxide, which can be found in its natural state as the ore smithsonite (ZnCO3; aka calamine or zinc spar) or sublimated and oxidised by intentionally roasting zinc-sulphide ores such as sphalerite (ZnS; aka zincblende) or zinc-containing fahlerz.1 Zinc oxide, or even droplets of zinc metal under extreme reducing condi-tions (cf. mock silver or false silver) can also be created acci-dentally when zinc ores get mixed up with copper or iron ores in a smelt, or with argentiferous lead ores during the produc-tion of lead or silver (Craddock and Eckstein 2003: 21718). In most cases, zinc oxide would be found by the metalworker as a white powder clinging to the inner lining of the furnace walls or in the flue (cf. Wertime 1980: 15). Given the rarity of naturally occurring zinc oxide ores in the Middle East and the ubiquity of mixed zinc-lead sulphide deposits, accidental production in a furnace seems highly probable as the source of ancient zinc oxide.2 The presence of lead slags bearing significant quanti-ties of zinc at sites such as 3rd-millennium BC Tepe Hissar in northeastern Iran (2.314.0 wt% zinc)3 and 1st-millennium BC Balya in northwestern Anatolia (3.230.3 wt% zinc) would seem to confirm this association (Pernicka et al. 1984; Pigott et al. 1982).
After producing or obtaining zinc oxide, the next step is to create a copper-zinc alloy by separating the zinc from the oxide through sublimation while adding it to copper before it re-oxidises. For the purposes of this paper, an alloy is defined as the intentional admixture of two or more elements in order to create a distinct material with certain desired physical prop-erties. Thus, while under extreme reducing conditions the accidental smelting of mixed ores or high-zinc copper ores can produce copper metal with as much as 67 wt% zinc (see Pollard and Heron 1996), this is not an intentional alloy per se. Certainly this type of low zinc copper-base metal has some desirable physical differences from pure copper that may or may not have been noticed by the metalworker. Intentionality is not certain, however, especially if we are only confronted with isolated examples for example the Early Cycladic dagger from Amorgos with 5.1 wt% zinc or the Middle Bronze Age axe from Beth-Shan with 6.5 wt% zinc mentioned by Craddock (1978a: 2). The addition of greater than ~8 wt% zinc produces a metal with at least one unmistakable char-acteristic its golden colour which, even if created fortui-tously the first time, probably could have been reproduced if desired. Therefore, copper-zinc alloys will be defined for this paper somewhat arbitrarily as containing greater than ~8 wt% zinc.
Before the intentional production of zinc metal through distillation processes, which according to texts seems to have begun in India in the late 1st millennium BC (Craddock et al. 1998), there were two basic ways to create copper-zinc alloys. The first is the cementation method, in which zinc oxide is mixed with pieces of copper metal and charcoal in a tightly closed crucible, heated above 906 C in order to vaporise the zinc and allow it to diffuse into the solid copper, before then introducing a final stage of raised temperature to melt the metal and thereby homogenise the mixture (Bayley 1998: 910). According to recent thinking (see Craddock and Eckstein 2003: 2236), the temperature range was probably closer to 10001100 C during Roman times, which would have pro-duced in one step a molten copper-zinc alloy of 2028 wt% zinc. Thilo Rehren (1999: 1085) has argued for a lower tem-perature range (c. 9001000 C) based on the material proper-ties of early ceramic crucibles, while Jean-Marie Welter (2003) has suggested an upper limit of zinc uptake closer to 3840 wt%. The amount of zinc in the resulting metal would also be significantly depleted if insufficient amounts of calamine were added to the mixture or if the base copper contained impurities such as tin or lead. In any case, subsequent melting of the copper-zinc alloy (or re-melting of scrap metal) would invariably cause the loss of about 10% of the zinc present in the alloy4 (Caley 1964).
The other way to achieve a copper-zinc alloy using zinc oxides, and the one perhaps more likely to have produced the prehistoric examples discussed in this paper, is through a mixed-ore smelting process. This method has been demon-strated by many scholars including Sun and Han (198385: 268), who managed to create copper-zinc alloys with up to 34 wt% zinc by mixing chemically pure zinc oxide (ZnO) and cuprous oxide (Cu2O) (1:1) in a graphite crucible. Of course, this was a modern smelting experiment and one not necessarily representative of ancient processes, but it should be noted that they also produced copper-zinc alloys (up to
O F B R A S S A N D B R O N Z E I N P R E H I S TO R I C S O U T H W E S T A S I A
18 wt% zinc) by smelting a mixture of naturally occurring malachite (Cu2(OH)2CO3) and leaded smithsonite. The effi-cacy of the mixed-ore smelting method was also supported by the work of Rostoker and Dvorak (1991), who produced a copper-zinc alloy of 10.5 wt% zinc by smelting zinc oxide with malachite in an open crucible, although they note that the zinc uptake would have been higher with a closed crucible. Although we do not as yet have a means of distinguishing these two general methods of copper-zinc alloy production using only the artefacts themselves, the mixed-ore smelting method (which here includes the mixture of copper ores with manmade zinc oxide) seems more likely to have been utilised, given what we know about prehistoric metallurgical processes in Southwest Asia.
Early copper-zinc alloys in Southwest Asia
Having delineated the possible means of copper-zinc alloy production in antiquity, it is time to turn to the evidence itself. As presented in Table 1, there are over 30 examples of prehistoric and protohistoric artefacts from Southwest Asia containing over 8 wt% zinc that have been reported in the literature. Also included are a number of artefacts containing 58 wt% zinc that may or may not be intentional alloys, but which are included here for the sake of reference. Notable finds east of the general area of Southwest Asia include the isolated and contested examples of copper-zinc alloys from the Yangshao and Longshan periods in central and eastern China (c. 4th3rd millennia BC) (see An 2000; Han and Ko 2000; Mei and Li 2003: 112; Sun and Han 198385). In addition, there are two leaded gunmetal artefacts from Atranjikhera, an early/mid-1st millennium BC site in the Upper Ganga Basin of northern India (Gaur 1983), which precede the leaded brass vessels from Taxila in northern Pakistan (4th century BC)
and Begram in the Kabul valley of Afghanistan (2nd century BC) (Craddock et al. 1998: 27). While the Chinese examples remain suspect because of their extreme discordance with the development of Chinese metallurgy as we understand it, the finds from Atranjikhera and elsewhere on the Indian subcontinent coincide with (or slightly predate) the earliest textual references to brass and possibly even zinc metal from this region (Craddock et al. 1998; see also Rau 1974).
Contemporary with the Indian examples, there are also sporadic examples of copper-zinc alloys from the Hellenistic world as well as textual references to oreichalkum (copper of the mountain; cf. Latin aurichalcum or golden copper),5 beginning as early as the 7th century BC (see Craddock 1998b; Craddock et al. 1980). Also of note from Europe are the 3rd-century BC Etruscan statues analysed by Craddock (1978b) that contain 11.5 and 11.8 wt% zinc (and 0.683.0 wt% tin respectively), the 6th-century BC pin with 9.9 wt% zinc from a Phoenician tomb in Cadiz, Spain (Montero-Ruiz and Perea, this volume, p. 136) and the pre-Roman iron sword with the makers stamps in brass (c. 1520 wt% zinc) from Syon Reach outside London now dated to the 2nd century BC (Craddock et al. 2004).6 These examples join the list of 21 prehistoric copper-zinc alloys compiled by Caley (1964: 38) in contesting the widely held belief that copper-zinc alloy production spread throughout Europe with the Roman conquests.
As stated above, the data from Southwest Asia can be grouped loosely into six spatially and chronologically defin-able clusters that predate the advent of the consistent utilisa-tion of copper-zinc alloys in the late 1st millennium BC (Fig. 2). The first of the six groupings (Group 1) is located in the eastern Aegean region during the first half of the 3rd millen-nium BC and includes the eight copper-zinc alloys presented by Stos-Gale (1992) and Begemann et al. (1992) from the site of Thermi on the island of Lesbos. Here one or two examples of copper-zinc alloys (c. 517 wt% zinc) were found in almost e...